ISSN Online: 2333-9721 ISSN Print: 2333-9705
DOI: 10.4236/oalib.1104390 Mar. 5, 2018 1 Open Access Library Journal
Analysis of the Motion of Frenkel-Kontorova
Dislocations in Single Crystals of Aluminum
with Allowance for the Peierls Barrier
Department of Physics, Yerevan State University, Yerevan, Armenia
The regularities of the motion of a one-dimensional Frenkel-Kontorova dis-location in pure aluminum at helium temperatures are studied. Computer si-mulation was carried out using the sine Gordon equation, written in dimen-sionless variables. It is proven that when the transition to dimendimen-sionless va-riables the discreteness of the model is preserved. The dependence of the true values of stresses on deformation in the Euler variables, as well as the velocity distribution of the dislocation fragments along the coordinate for successive instants of time, are obtained. It is shown that under these conditions disloca-tion modisloca-tion is realized by quantum tunneling of the dislocadisloca-tion bends. The quantum-mechanical estimate confirms the possibility of quantum tunneling of the kink of dislocations in aluminum at low temperatures.
Mechanics, Modern Physics
Aluminum, Frenkel-Kontorova Dislocation, Sine Gordon Equation, Computer Simulation, Dislocation Kinks, Quantum Tunneling
Many elements of modern technology operate under conditions of moderate (up to 200 K) and deep (up to 4 K) cooling. These are elements of liquefaction and separation plants, spacecraft systems, etc. It was found that with decreasing temperature most of the metals become more durable. At 77 K (the boiling point of liquid nitrogen), the strength of copper is doubled, and the strength of alu-How to cite this paper: Arakelyan, M.
(2018) Analysis of the Motion of Frenkel-Kontorova Dislocations in Single Crystals of Aluminum with Allowance for the Peierls Barrier. Open Access Library Journal, 5: e4390.
Received: February 1, 2018 Accepted: March 2, 2018 Published: March 5, 2018
Copyright © 2018 by author and Open Access Library Inc.
This work is licensed under the Creative Commons Attribution International License (CC BY 4.0).
DOI: 10.4236/oalib.1104390 2 Open Access Library Journal minum is six times larger than at room temperature. At low temperatures, espe-cially under load, internal structural transformations occur, which increases the risk of sudden destruction of products. The transition of metals into a fragile state at low temperatures is associated with a change in the plasticity characteris-tics. Investigations of the physical nature of the problem show that the transition to the fragile state of pure single crystal samples depends on temperature, rate of deformation, dislocation density, etc.
Although a large number of studies are being carried out in this direction, for example  , the developed physical models do not allow to quantify the in-fluence of numerous factors. A number of questions remain unclear, in particu-lar, the problem of an abnormal decrease in the plastic flow stress in aluminum at low temperatures.
Therefore, a study of the nature of the change in the strength and plasticity parameters of metals as a function of temperature and deformation rate at tem-peratures from 293 K to the boiling point of liquid helium (4.2 K) is of great scientific interest.
2. Theoretical Background
In the plastic region, unlike the elastic region, qualitatively new physical pheno-mena are realized. If a volume change occurs in the elastic region with a change in the stress state, then the physics of the phenomenon changes radically in the region of plasticity. Dislocations move under the condition that the volume is constant, and the dependence of the yield stress on the accumulated deformation has a nonlinear character. For most deformable metals, the transition from elas-ticity to the plaselas-ticity region is of a smooth nature, so a 0.2% residual deforma-tion is considered as the condideforma-tional boundary of such a transideforma-tion, and the cor-responding stress is called the conditional yield point. Therefore, in the region of plasticity, conditions for the constancy of volume are used to obtain the stress-strain relation . For sufficiently large plastic deformations, to compare the results of the theory with experiment, the conditional values of stresses and deformations go to their real values.
In  the nonlinear dependence of the yield stress on the accumulated defor-mation, strain rate and temperature is
3 1 2
σ= ε ζ − (1)
0 3.6 10 MPa, 1 0.255, 2 0.05, 3 0.01
a = × a = a = a = − , a a a a0, ,1 2, 3-constants of material, ζ-rate of deformation, θ-temperature on Celsius scale.
DOI: 10.4236/oalib.1104390 3 Open Access Library Journal the remaining part of the dislocation there.
It follows from the deformation diagram  that, beginning with the strength limit of the material, when the deformation increases, its localization takes place, the active stress increases intensively and the sample breaks down. However, if a sharp decrease in the true stress occurs at stresses below the true value of the tensile strength, the interpretation of this result requires additional assumptions.
The simulation was carried out using sine Gordon equation for the one-dimensional Frenkel-Kontorova dislocation model. In the Frenkel-Kontorova model, the atoms above the glide plane are material points connected by springs of rigidity «k», and the atoms under the glide plane (substrate) are described by a sinusoidal potential. The Frenkel-Kontorova model is discrete and this is its ad-vantage over other models. Within the framework of the chosen model, the mo-tion of dislocamo-tions is described by the sine Gordon equamo-tion.
0sin 2π 1 1 2
n n n n n
my = −f y a +k y+ +y− − y (2)
where yn is deviation of the n-th atom from the equilibrium position, a-lattice constant, f0sin 2
)-periodic sinusoidal force on the substrate side, m-mass of the atom, k-stiffness coefficient.
In dimensionless units, the sine Gordon equation takes the form:
n n n
ϕ + ϕ ϕ′′− = (3)
where ϕn is displacement n-th atom from the equilibrium position.
When changing to dimensionless variables, finite differences are replaced by spatial derivatives. However, the discreteness of the model is preserved. We will carry out the corresponding analysis. The dislocation size is determined as fol-lows :
2 0 0 2π0
l =a mv f a
v =a k m-speed of sound, l0-size of dislocation, a-inter-atomic distance.
The denominator is the product of the force at a distance, which is obviously proportional to the work that must be spent on overcoming the Peierls barrier separating one valley from the other. Thus, it increases with increasing spring stiffness and decreasing forces on the substrate side. Assuming that the elastic energy greatly exceeds the work, we obtain that l0a. It follows from the condition obtained that we are considering the case of the long-wave approxi-mation. Using the sine Gordon Equation (3), we model the displacement field, the deformation field, and the stress field near the dislocation.
DOI: 10.4236/oalib.1104390 4 Open Access Library Journal (a)
Figure 1. The displacement field of the dislocation (a) and the stress field around the
In particular cases, the sine Gordon equation admits the solution in an ana-lytical form. In more complex cases, approximate solutions of the inhomogene-ous sine Gordon equation are obtained using perturbation theory (e.g. ). We investigate solutions of the inhomogeneous sine Gordon equation in numerical form.
The initial conditions were taken by us, using a known analytical solution of the homogeneous sine Gordon equation at the initial instant of time. The sim-plest boundary conditions, which have a physical meaning, consist in the fact that the sample through which the dislocation propagates is considered open at both ends,
x x l
∂ ∂ = ∂ ∂ =
where l-dimensionless sample length.
There are two equivalent approaches when considering the motion of a de-formable material: the Euler approach and the Lagrange approach. When atten-tion is concentrated on a given point in space into which different particles of a deformed medium come, this is the Eulerian approach. Movement from the Eu-lerian point of view is known if speed, acceleration, temperature, etc. are given as functions of coordinates of a given point of space and time-these are Euler va-riables. When attention is concentrated on a particular particle of the medium and the history of its deformation and motion is studied, this is the Lagrange
-15 -10 -5 5 10 15
DOI: 10.4236/oalib.1104390 5 Open Access Library Journal approach. The choice of the kind of variables is made on the basis of the nature of the problem to be solved. We solve the problem using Euler’s approach.
The problem was solved by us in the Eulerian analysis for the following rea-sons. Under the Eulerian approach, we study the characteristics of the change in the field of a moving dislocation at a given point in space over time. In the La-grange case, the evolution of the motion in the space of a given point of the dis-location field is investigated.
The nonlinear differential sine Gordon equation, with which we describe the motion of dislocations, is also used in the description of weak superconductiv-ity in the Josephson tunnel junction between two closely located supercon-ductors. In addition, for certain values of the parameters it goes over into the Klein-Gordon equation, which is a quantum equation. Therefore, we assumed that the phenomenon of tunneling of inflections can be described by a sine Gordon’s equation.
3. Results. Discussion
By numerically solving the sine Gordon Equation (3), using the initial and boundary conditions given above, we get the dependence ϕn
( )x t, . Next, from the displacement function, we go to deformations, then using the experimentally obtained (describing the true stresses and deformations) dependence of me-chanical stress on deformation, deformation rate and temperature (1), we find the dependence of the true stresses on deformation in aluminum at helium tem-peratures in Euler variables Figure 3(a).
As is known, the conditional tensile strength for aluminum is 8 × 108
Using a known relationship between true and conditional stresses
σ =σ +ε , for the true value of the tensile strength, we obtain the
8 10 1× +
εdyne/cm2, where ε-the coordinate of the abscissa at the
beginning of the descent. If the values of σn, at which the curve starts to go
8 10 1
σ< × +
ε, then the tunneling effect occurs, if at any of these
points the value σn is greater than the true value of the tensile strength, then deformation is localized and the sample is destroyed.
From the data of the numerical experiment (Figure 3(a)) we calculated the true values of stresses and deformations at which a sharp softening occurs (the descents on the curve), and compared the obtained values of the stresses at these points with the true value of the aluminum tensile strength (Table 1).
As a result, we can conclude that in our numerical experiment at points of sharp softening (points (1-6) in Figure 3(a)), the crystal fracture cannot happen, the stress values at these points are less than the true value of the tensile strength. It follows from the numerical experiment (Figure 3(b)) that the veloc-ity of dislocation movement relative to the medium is periodic.
DOI: 10.4236/oalib.1104390 6 Open Access Library Journal
Table 1. True values of stresses and deformations at which a sharp softening occurs and
the true value of the tensile strength.
ε σ 8 × 108 (1 + ε)
1 0.185 2.73 × 106 9.48 × 108
2 0.254 2.94 × 106 10.032 × 108
3 0.267 3.06 × 106 10.136 × 108
4 0.288 3.1 × 106 10.304 × 108
5 0.358 3.26 × 106 10.864 × 108
6 0.465 3.42 × 106 11.72 × 108
the medium from the side of the Peierls barrier. The consequence of this is an increase in stress. When the dislocation falls into the valley of the potential Peierls relief, the resistance to movement of the dislocation decreases sharply, as a result of which the stress is relaxed (softening) and the sign of the dislocation velocity reverses. Thus, when the Peierls barrier is overcome, the dislocation moves, slowing down before the barrier and accelerating after overcoming the barrier (3b), i.e. processes of micro-hardening and micro-softening occur pe-riodically. Consequently, the nature of the stress variation in the vicinity of the investigated region (near the dislocation) reflects the above-mentioned character of the dislocation motion (Figure 3(c)), caused by the discrete nature of the me-dium: the softening has an almost periodic character.
We assume that a sharp decrease in the stress with an almost constant defor-mation, which is periodic in nature, can be explained by tunneling of kinks through the Peierls potentials.
From this point of view, the result presented in Figure 3(a) can be explained as follows. When a dislocation moves, a stress field is created around it, that re-flects the nature of the evolution of the medium properties. When the Peierls barrier is overcome, the dislocation moves jump wise, slowing down before the Peierls barrier and accelerating after overcoming the barrier (Figure 4). Because of this, the nature of the stress variation in the vicinity of the investigated region (near the dislocation) reflects the above-mentioned dislocation movement pat-tern, caused by the discreteness of the medium: softening (tunneling) has a pe-riodic character, which correlates with the oscillating dependence of the defor-mation on the coordinate (Figure 2(b) and Figure 2(c)), the growth of the curve
σ ε is nonlinear.
As can be seen from Figure 3 and Figure 4, the tunneling process, as ex-pected, is non stationary.
DOI: 10.4236/oalib.1104390 7 Open Access Library Journal (a)
Figure 2. The dislocation displacement field (a), the deformation field to the right of the
dislocation (b), the deformation field to the left of the dislocation (c).
It is known that in aluminum at low temperatures an abnormally high creep rate is observed, which in the literature   is interpreted on the basis of quantum-mechanical models. In metals at low temperatures dislocation motion is ensured by moving relatively small distances of a large number of small-scale fragments. In aluminum samples, only the kinks of dislocations can be noticea-ble mobility, which can be regarded as point defects (quasiparticles) on disloca-tions. It is known from quantum mechanics that the tunneling condition for a quasiparticle through a potential barrier has the form 2 2m Ws
DOI: 10.4236/oalib.1104390 8 Open Access Library Journal (a)
Figure 3. (a) The stress-strain dependencein the Euler variables; (b) Dependence of
dis-location velocity on time for the same time intervals; (c) The dependence of the stress on time in the vicinity of the dislocation for the same time intervals.
(-Planck’s constant, ms-effective kink mass). Calculations give that for kinks in aluminum 2 2m Ws
, which confirms the possibility of
tunneling of kinks.
DOI: 10.4236/oalib.1104390 9 Open Access Library Journal t1
Figure 4. The displacement field of a dislocation moving by way of kinks tunneling, and
the coordinate distribution of velocities of the same dislocation (a bold line) for succes-sive instants of time.
-15 -10 -5 5 10 15 x
-6 -4 -2 2 4 6 8 10 v
-15 -10 -5 5 10 15 x
-6 -4 -2 2 4 6 8 10 v
-15 -10 -5 5 10 15 x
-6 -4 -2 2 4 6 8 10 v
-15 -10 -5 5 10 15 x
DOI: 10.4236/oalib.1104390 10 Open Access Library Journal
( )1 2
h mu a ∆
ais the inter atomic distance, m is the mass of atoms, and u is the ener-gy of interaction of neighboring atoms. For most crystals the parameter Δ is very small. In quantum crystals
~ 1and the delocalization effect of particles is
significant. Because of the smallness of the mass of the kinks and their weak in-teraction with the matrix atoms, the kink can be delocalized in the crystal, while the atoms of the matrix themselves behave in a classical way.
Calculations show that in aluminum, 14
u − and Δ ≈ 0.4 (for
compar-ison, in quantum crystals for He3, Δ ≈ 0.49, for neon Δ ≈ 0.07. In all pure metals
the parameter Δ is negligibly small ).
The result obtained speaks in favor of the fact that tunneling is possible.
Thus, numerical modeling, theoretical estimation and comparison with experi-ment allow us to conclude that in pure aluminum (99.9998%) at low tempera-tures (4.2 K) the anomalously high creep rate can be explained by quantum tunneling of the dislocation kinks.
 Malygin, G.A. (1999) Dislocation Self-Organization Processes and Crystal Plasticity.
Physics-Uspekhi, 42, 887-916.
 Malygin, G.A. (2007) Plasticity and Strength of Micro- and Nanocrystalline Mate-rials. Physics of the Solid State, 49, 1013-1033.
 Hosford, W.F. and Caddell, R.M. (2007) Metal Forming: Mechanics and Metallurgy. 3rd Edition, Cambridge University Press, Cambridge, 330 p.
 Zagirov, N.N. (1998) Theoretical Foundations of Plastic Deformation. Krasnoyarsk, 120 p.
 Melik-Shakhnazarov, V.A., Mirzoeva, I.I. and Naskidashvili, I.A. (1986) Tunneling of Dislocation Kinks in Aluminum. JETP Letters, 43, 316-319.
 Hirth, J. and Lothe, J. (1972) Theory of Dislocations. McGraw-Hill Book Company, Institute of Physics, Oslo University, New York, 599 p.
 Fogel, M.B., Trullinger, S.E., Bishop, A.R. and Krumhans, J.A. (1977) Dynamics of sine-Gordon Solitons in the Presence of Perturbations. Physical Review B, 15, 1578.
 Estrin, Y.Z., Isaev, N.V., Grigorova, T.V., Pustovalov, V.V., Fomenko, V.S., Shumi-lin, S.E., Braude, I.S., Malykhin, S.V., Reshetnyak, M.V. and Janecek, M. (2008) Low-Temperature Plastic Deformation of Ultrafine-Grained Aluminum. Low Temperature Physics,34, 665-671.https://doi.org/10.1063/1.2967513
DOI: 10.4236/oalib.1104390 11 Open Access Library Journal
 Petukhov, B.V. (1985) The Theory of Low-Temperature Plastic Strain Anomalies Caused by Tunneling of Kinks. Fizika Metallov i Metallowedenie, 60, 255-261.  Petukhov, B.V. and Pokrovsky, V.L. (1972) Quantum and Classical Motion of
Dis-locations in a Pejerls Potential Relief. JETF, 36, 336-342.